- About this Journal ·
- Abstracting and Indexing ·
- Aims and Scope ·
- Article Processing Charges ·
- Articles in Press ·
- Author Guidelines ·
- Bibliographic Information ·
- Citations to this Journal ·
- Contact Information ·
- Editorial Board ·
- Editorial Workflow ·
- Free eTOC Alerts ·
- Publication Ethics ·
- Reviewers Acknowledgment ·
- Submit a Manuscript ·
- Subscription Information ·
- Table of Contents

International Journal of Optics

Volume 2012 (2012), Article ID 606892, 11 pages

http://dx.doi.org/10.1155/2012/606892

## Parametric Conversion in Micrometer and Submicrometer Structured Ferroelectric Crystals by Surface Poling

^{1}DIEET, University of Palermo, Viale delle Scienze, Building no. 9, 90128 Palermo, Italy^{2}Nonlinear Optics and OptoElectronics Laboratory (NooEL), University Roma Tre, Via della Vasca Navale 84, 00146 Rome, Italy

Received 27 July 2011; Accepted 26 September 2011

Academic Editor: Arnaud Mussot

Copyright © 2012 Alessandro C. Busacca et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

#### Abstract

We report on recent technological improvements concerning nonlinear patterning of lithium niobate and lithium tantalate in the micrometer and submicrometer scales using surface periodic poling for ferroelectric domain inversion. The fabricated samples were employed for frequency doubling via quasiphase-matching both in bulk and guided wave geometries, including forward and backward configurations and wavelength conversion in bands C and L. We also investigated short-period quasiperiodic samples with randomly distributed mark-to-space ratios.

#### 1. Introduction

Optical frequency conversion in parametric media is one of the most important applications in nonlinear optics, as it allows generating coherent light in regions of the spectrum where laser emission is not available. Moreover, through a careful engineering of the phase mismatch and excitation(s), several signal processing schemes can benefit of parametric nonlinearities via cascading [1–7]. Since the first experiments on second-harmonic generation (SHG) [8–10], a great effort has been devoted towards developing configurations with the highest conversion efficiencies [11, 12]. Among them, quasi-phase matching (QPM) is one of the most useful and versatile techniques for efficient frequency conversion, allowing continuous growth of the generated wave along the propagation length despite the local phase velocity mismatch (hence, lack of momentum conservation) between the interacting waves [13, 14]. This can be achieved thanks to a correction of their relative phases by means of a structural periodicity built in the nonlinear medium; more precisely, a periodic sign change of the quadratic coefficient as it can be achieved in noncentrosymmetric crystals, for example, lithium niobate (LN) and lithium tantalate (LT), via periodic poling (PP). Several techniques have been developed for PP, including domain inversion during crystal growth [15], spontaneous Curie temperature poling using heat [16], chemical reactions or substitution of impurities [17, 18], electron beam [19–22], and electric field assistance [23–25]. In recent years, surface periodic poling (SPP) was introduced as a PP approach for the fine tuning of the mark-to-space ratios in short-period QPM, aiming at the realization of smaller and smaller domain lengths for sum-frequency generation at shorter wavelengths, as well as backward or counterpropagating wave mixing [26–36]. Surface periodic poling is based on the overpoling of a ferroelectric substrate and provides periodic domain inversion with shallow domain depths as compared to the thickness of the substrate [30]. Short domains are also useful for broadband SHG: once the nonlinear (QPM) grating is fabricated, irregularities of the periodic structure lead to a random distribution of the mark-to-space ratio (MTSR) which has a relevant role when the desired pattern has small features (Figure 1(a)). The random modulation of the nonlinear coefficient allows phase matching between the fundamental (FF) and the SH beam thanks to the presence of several reciprocal lattice vectors (see Figure 1(b)), and, even far away from the QPM-SHG resonance, the harmonic signal remains remarkably large as compared to that generated in unpoled regions. While the SH output profile in space becomes strongly dependent on the wavelength (in the absence of effective self-focusing via cascading [37–40]), the randomized quasiphase matching (rQPM) process is quite broadband [41–44].

In this paper, we review some of the most recent technological improvements on QPM patterning of LN and LT in the micrometer and submicrometer scale. The fabricated samples were tested and used for parametric frequency doubling and difference frequency generation (DFG) via bulk and guided wave parametric interactions, including forward and backward configurations. We also characterized the rQPM interaction for SHG.

#### 2. Sample Fabrication

In order to achieve QPM and efficient parametric interactions for frequency conversion, domain inversion at the required period needs to be implemented. In some applications, such as first-order forward-SHG in LN and LT from fundamental wavelengths in the C band of optical communications, typical periods amount to about 20 *μ*m [45–47]. For other scopes, such as UV generation or backward-SHG, shorter periods are required: UV generation via frequency doubling can be achieved by employing periods of a few microns [48], while backward-SHG (at low order QPM) needs submicron periods [49–53]. Adopting the SPP approach, we were able to fabricate ferroelectric samples with periods in the micron and submicron range [30, 32, 54, 55].

The samples were prepared from standard optical grade wafer substrates of congruent LN or LT of thickness 500 *μ*m [54, 56]. For SPP we used high-voltage pulses applied across the thickness in order to achieve overpoling. We spin coated the − face of the crystal slab with a photoresist film (Shipley S1813) and defined the desired periodic pattern by standard photolithography. After development, the pattern was soft baked overnight at 90°C and hard baked at 130°C for 3 hours. The temperature was raised gradually in order to avoid problems due to pyroelectric effects, the formation of poling dots, and the insurgence of mechanical stress in the bulk. The baked photolithographic mask served as the insulating layer during high-voltage poling for producing domain inversion, although SPP was also occasionally carried out with the aid of photolithographically defined silica masks, the latter improving the duty cycle control with 50 : 50 MTSR [32].

The samples were then placed between two electrodes covered with a thin gel electrolyte to ensure proper electric contact. Hence, the LT (or LN) interfaces were connected to a high-voltage waveform generator (Agilent 3220 A) after amplification (Trek 662). A digital oscilloscope helped monitoring the waveforms of both the poling voltage and the displacement current.

To exceed the coercive field in the ferroelectric crystals and obtain surface periodic inversion, we applied 1.3 kV pulses over a 10 kV bias for an appropriate time interval, in order to fulfill the overpoling condition: with the flowing charge, the poled area, and the spontaneous polarization of the material. With this approach, even without a precise control of the flowing charge, one can allow the domain walls to completely merge on the face of the crystal but not underneath the insulated portions of the face, where the original ferroelectric orientation gets preserved in a periodic fashion (see Figure 2). We could evaluate the domain uniformity, depth, and MTSR by etching the poled samples in diluted hydrofluoric acid (HF, 50%) and investigating the periodic grating by a scanning electron microscope (SEM).

Submicron gratings were written on a photoresist mask by means of an interferometric pattern obtained with the 441.6 nm light emitted by a He-Cd laser. The samples, coated with a 400 nm thick spun photoresist (Shipley S1805), were arranged in the Lloyd configuration with a mirror orthogonal to the surface (see Figure 3). The 6 mW He-Cd beam was expanded and collimated to the sample-mirror system, one half being reflected and forming interference fringes with period with the other half, being , the angle between the beam and the normal to the sample, as set by a rotation stage. The exposure time was about 15 s. Since LN and LT are transparent in the near UV, we also covered the sample back face with a matching index liquid in order to minimize the detrimental effects of multiple reflections on the fringe visibility. After exposure, the photoresist development was checked by measuring the grating diffraction efficiency under He-Ne laser illumination. We were able to produce good quality 400 nm period gratings that were employed as insulating masks during SPP [56].

Table 1 summarizes the technological details for various samples. Figure 4 displays the scanning electron microphotographs of typical periodic QPM gratings.

In order to enhance the parametric conversion efficiency, we often resorted to fabricating optical waveguides; this ensured tightly confined interacting waves over the whole propagation length and, therefore, higher and nearly constant intensities with respect to bulk, where diffraction occurs.

Among the available techniques for waveguide fabrication, we chose proton exchange (PE) in the *α*-phase [57], as it preserves the nonlinear properties of the crystal and is compatible with the electric field poling of the ferroelectric domains in both LN and LT [58–60]. The poled substrates were initially coated with a SiO_{2} layer; channel openings, typically from 1 to 7 *μ*m in width, were defined by standard photolithography and wet etching in HF (Figure 5(a)). Proton exchange was then carried out by dipping the LN/LT sample in a solution of benzoic acid (BA) and 3–3.6% lithium benzoate (LB) using the sealed-ampoule method [60], as sketched in Figure 5(b). This yielded an extraordinary refractive index increase and low proton concentration (*α*-phase) channel waveguides supporting TM-polarized modes. We verified the compatibility between SPP and PE by chemically etching the samples and using scanning electron microscopy as well as by performing nonlinear measurements in guided-wave configurations [46, 48, 61]. Figure 4(c) shows the optical micrograph of a typical channel on a PP substrate after HF etching.

We also employed planar waveguides formed on the face of the samples for distributed prism coupling and the evaluation of the extraordinary index profile versus depth using the standard WKB method [62]. Figure 5(c) shows an example of such a profile in a PE-SPPLN waveguide fabricated by using a solution of BA + 3% LB and proton exchange at 300°C for 96 hours.

#### 3. Parametric Characterization

After fabrication, our samples were nonlinearly characterized and tested: the inversion of the quadratic coefficient with different periods allowed us to achieve efficient parametric frequency doubling at the corresponding QPM resonant wavelength in each configuration (forward or backward) or to obtain broadband SHG via randomized QPM. Hereby, we report on typical experimental results obtained either in bulk or in channels from three different samples with micron-scale domain inversion.

The first sample was a PPLN bulk with a one-dimensional grating of period 3.2 *μ*m over a length of 3 mm. For the nonlinear measurements, we used an Argon-ion pumped CW Ti: Sapphire laser, with a 40 GHz linewidth and wavelength tunable between 860 and 1000 nm; with an lens, the TEM_{00} beam was gently focused to a waist of 30 *μ*m in the middle of the poled area, in a crystal kept at a constant temperature of 195°C to reduce or prevent the risk of photorefractive damage. The FF beam was mechanically chopped at 133 Hz, and the generated SH signal was collected by a photomultiplier tube for synchronous detection; the residual pump was eliminated with the aid of a dichroic mirror and selective bandpass filters. Initially, we studied the SH generated forward via first-order QPM by light at . We spectrally resolved the QPM-SHG resonance by varying either the FF wavelength (Figure 6(a)) or the temperature (Figure 6(b)) while keeping the other parameters constant. We then verified the quadratic growth of the SH versus FF excitation (Figure 6(c)). BSHG measurements were also performed on the same sample, and Figure 7(a) shows the normalized BSHG conversion efficiency versus input FF wavelength for the 29th and 30th grating orders of QPM-BSHG. The presence of frequency-doubled light at both odd and even resonant orders is attributed to the unbalanced duty cycle. The BSHG power at resonance grew quadratically with FF excitation; Figure 7(b) shows the normalized BSHG conversion efficiency (30th order) versus temperature, the latter permitting the fine tuning of the resonance. The 30th resonant order resulted to be the most efficient as we obtained up to 17.2 pW of backward SH power by using an FF excitation of 55.12 mW, corresponding to a maximum conversion efficiency . Considering an effective length of 0.5 mm for the grating [53], the maximum normalized efficiency is . This value is remarkably high if compared to what obtained in similar LN samples with a 3.3 *μ*m poling period. For example, in [49], a normalized efficiency of 7·10^{−9}% W^{−1} cm^{−1} was achieved by exciting the sample in the fs regime at a lower resonant order (17th). Moreover, the maximum efficiency we got is of the same order of magnitude of what reported in [50] by using a ns source to excite the 16th resonant order: for a pump power of 33.75 kW and an interaction length of 4 mm, corresponding to a normalized efficiency .

The second sample consisted of PE channel waveguides fabricated on a LT substrate with a 10 mm long 2.0 *μ*m periodic pattern for QPM. For the characterization, we used the same source described above, with the beam end-fire coupled to the channels by a 10x microscope objective, keeping the sample at a constant temperature of 250 ± 0.1°C against photorefractive damage.

A filter at the waveguide output helped eliminating the fundamental frequency pump in the near infrared, and another filter suppressed the remaining Argon-ion light. The generated SH power in the UV was measured with a calibrated Silicon photodiode, with a mechanical chopper and a lock-in amplifier to reduce the noise level.

Figure 8 plots the generated SH power versus input FF wavelength in 7 *μ*m wide channels: the SHG resonance occurred between fundamental order TM modes for an input wavelength close to 730.7 nm. These *α*-phase PE SPP-LT waveguides, featuring a short 2.0 *μ*m QPM period, were the first coherent integrated optics UV parametric sources at 365.4 nm, with remarkably high conversion efficiencies exceeding 7.5% W^{−1} cm^{−2} [48]. The latter value is comparable to what reported in [63], where a normalized conversion efficiency of 8.4% W^{−1} cm^{−2} was achieved for SHG with FF in the C-band of optical communications using reverse-PE optical waveguides in PP stoichiometric LT (definitely more expensive than congruent LT). Similar results were achieved in alpha-phase PE channel waveguides with electric field SPP of congruent lithium niobate crystals: we obtained UV SHG at 390 nm via first-order QPM by the fabrication of periodic structures with a pitch as small as 750 nm [64].

On the same sample but in a bulk configuration, we also performed broadband SHG via rQPM far from the resonance. When exciting the sample with a Gaussian beam at the resonant FF wavelength, we obtained at the output a bell-shaped SH profile across the whole domain-inverted substrate. This stems from first-order QPM in bulk, due to the 2.0 *μ*m periodicity in the () quadratic nonlinearity; however, wavelength detunings as small as 1 nm abruptly caused the SH level to drop down at the level of the background noise. The random-QPM contribution manifested at FF wavelengths above 900 nm, where we could observe larger SH powers increasing with FF wavelength: the parabolic increase versus input FF power at is clearly visible in Figure 9(a). This rQPM-SHG process exhibited a conversion efficiency of about 4·10^{−5}% W^{−1} cm^{−1}, about 1 order of magnitude lower than at resonance and more than one order of magnitude higher than what reported in [65], where a similar configuration was explored in Sr_{x}Ba_{1-x}Nb_{2}O_{6} crystals. The near-field CCD images of the SH showed a random set of finger-like features, parallel to one another and to the axis, with intensities and distributions strongly depending on location and wavelength of the input FF beam. The nonresonant trend of the SHG is characteristic of rQPM and is shown in Figure 9(b), graphing SH conversion efficiency versus FF wavelength [41].

Finally, we used the slab waveguide on the facet of the same sample for experiments on parametric beam self-trapping (via cascading) in the presence of rQPM. Since high intensities are required for this kind of experiments, in order to avoid photorefractive damage, we used a pulsed source with a low repetition rate. We employed 25 ps pulses from a 10 Hz parametric generator tunable in the near-IR with a linewidth ≤2 cm^{−1}. The beam was filtered to the TEM_{00} mode and adjusted in polarization and peak power. We monitored energy and peak power with a boxcar averager, filtering out fluctuations greater than 10%. We investigated the out-of-resonance response in the interval 980–995 nm. The FF beam was focused to a waist of 4 *μ*m along × 15 *μ*m along at the input facet of the planar PP-LT waveguide, ensuring a propagation length >6 Rayleigh distances. At low powers, we still observed randomly distributed SH with patterns along strongly dependent on both FF wavelength and input position, as previously discussed in the cw case. At high excitations, quadratic solitons are expected in upconversion (i.e., with an FF input) for wavelengths longer than the resonant one, corresponding to a positive phase mismatch. At high powers, we noticed a progressive reduction in FF size at the output, with waists of about 130 *μ*m along in the quasilinear regime and of 37 *μ*m at peak excitations >100 kW [40]. A similar trend was detected for the envelope of the “speckled” SH signal, owing to randomness and off-axis nonlinear scattering. Figure 10 displays a selection of both FF and SH output beams, for various FF input peak powers. Clearly, self-focusing of both FF and SHG beams is observed for increasing FF, suggesting the formation of a two-color spatial solitary wave (simulton) in one transverse dimension. Figure 11 graphs the output FF spot size versus input peak power at both 991 and 985 nm: such behavior is predicted by the model detailed in [40], as well. The agreement between model and experimental results confirms that self-localization takes place via quadratic cascading [38].

The third sample we report on consists in PE channel waveguides in periodically poled congruent LT (PPLT) with period 20.8 *μ*m and a propagation length of 2.25 cm. The waveguides, from 8 to 13 *μ*m wide, were fabricated as described in the previous section and resulted single mode at telecom wavelengths [61]. The nonlinear characterization was carried out at room temperature with a wavelength tunable external-cavity laser (ECL) linearly polarized and butt-coupled to the waveguides in order to excite TM modes; we used micropositioners and standard single-mode fibers with an effective area and propagation losses at 1550 nm. The output light was collected by either a microscope objective or fiber end-fire coupling, depending on the measured quantity. The overall (fiber to fiber) insertion losses in the waveguide amounted to 7 dB. From our measurements, the coupling losses at each waveguide facet were 1.2 dB; hence, we estimated the propagation losses in about 2 dB cm^{−1}. Using a fundamental frequency beam in the TM polarization from the ECL, we first characterized QPM-SHG at the resonances of the FF TM_{00} mode with the various TM modes supported at the SH. By tuning the FF, we achieved quasi-phase matching at three wavelengths (Figure 12(a)): the resonance at 1566.90 nm corresponds to the interaction between FF TM_{00} and SH TM_{00}; those at 1555.43 and 1552.29 nm are due to QPM between the FF TM_{00} and SH higher-order modes. Because of the modal profiles in the graded index channel, the highest conversion efficiency was achieved between FF TM_{00} and the fourth SH mode (Figure 12(a)). We then tested the device as an all-optical wavelength converter (AOWC) based on quadratic cascading [66], by input coupling two copropagating continuous wave beams at distinct wavelengths in the C-band. Both inputs were amplified in erbium-doped fibre amplifiers, filtered (to rid of the out-of-band noise), and butt-coupled with a 90/10 fibre coupler. Their linear polarization was adjusted to match the -axis of the PPLT. The pump beam was set at the phase matching for SHG (), and the probe was detuned by nm (). The coupled optical powers were about 100 and 15 mW for pump and probe, respectively. By cascading SHG and DFG, the device generated a downshifted signal () with power larger than 100 nW (Figure 12(b)), demonstrating for the first time both wave confinement and two-stage parametric conversion in LT channels at wavelengths around 1.5 *μ*m [45].

#### 4. Conclusions

In conclusion, we summarized both the technological steps for sample fabrication by surface periodic poling and waveguide fabrication by proton exchange on ferroelectric substrates, namely, lithium tantalate and lithium niobate. The optical characterization of these micro- and nanoengineered devices, both in bulk and in guided-wave configurations, shows the high potentials of the adopted technology towards forward and backward parametric generation, down to the UV, as well as towards cascaded wavelength shifters operating in the C and L bands. Moreover, we demonstrated that a randomized mark-to-space QPM ratio allows to obtain broadband frequency doublers with appreciable conversion efficiencies and, at higher intensities, parametric self-trapping via quadratic cascading.

#### References

- R. De Salvo, D. J. Hagan, M. Sheik-Bahae, G. Stegeman, E. W. Van Stryland, and H. Vanherzeele, “Self-focusing and self-defocusing by cascaded secondorder effects in KTP,”
*Optics Letters*, vol. 17, pp. 28–30, 1992. View at Google Scholar - G. I. Stegeman, M. Sheik-Bahae, E. Van Stryland, and G. Assanto, “Large nonlinear phase shifts in second-order nonlinear-optical processes,”
*Optics Letters*, vol. 18, no. 1, pp. 13–15, 1993. View at Google Scholar · View at Scopus - G. Assanto, G. Stegeman, M. Sheik-Bahae, and E. Van Stryland, “All-optical switching devices based on large nonlinear phase shifts from second harmonic generation,”
*Applied Physics Letters*, vol. 62, no. 12, pp. 1323–1325, 1993. View at Publisher · View at Google Scholar · View at Scopus - G. Assanto, I. Torelli, and S. Trillo, “All-optical processing by means of vectorial interactions in second-order cascading: novel approaches,”
*Optics Letters*, vol. 19, no. 21, pp. 1720–1722, 1994. View at Google Scholar · View at Scopus - D. J. Hagan, Z. Wang, G. Stegeman, E. W. Van Stryland, M. Sheik-Bahae, and G. Assanto, “Phase-controlled transistor action by cascading of second-order nonlinearities in KTP,”
*Optics Letters*, vol. 19, no. 17, pp. 1305–1307, 1994. View at Google Scholar · View at Scopus - G. Assanto, “Transistor action through nonlinear cascading in Type II interactions,”
*Optics Letters*, vol. 20, no. 15, pp. 1595–1597, 1995. View at Google Scholar - G. Assanto, Z. Wang, D. J. Hagan, and E. W. Vanstryland, “All-optical modulation via nonlinear cascading in type II second-harmonic generation,”
*Applied Physics Letters*, vol. 67, pp. 2120–2122, 1995. View at Publisher · View at Google Scholar · View at Scopus - P. A. Franken, A. E. Hill, C. W. Peters, and G. Weinreich, “Generation of optical harmonics,”
*Physical Review Letters*, vol. 7, no. 4, pp. 118–119, 1961. View at Publisher · View at Google Scholar · View at Scopus - A. Savage and R. C. Miller, “Measurements of second harmonic generation of the ruby laser line in piezoelectric crystals,”
*Applied Optics*, vol. 1, no. 5, pp. 661–664, 1962. View at Google Scholar - A. Ashkin, G. D. Boyd, and J. M. Dziedzic, “Optical second harmonic generation and mixing,”
*IEEE Journal of Quantum Electronics*, vol. 2, no. 6, pp. 109–124, 1966. View at Google Scholar - Y. J. Ding and J. B. Khurgin, “Second-harmonic generation based on quasi-phase matching: a novel configuration,”
*Optics Letters*, vol. 21, no. 18, pp. 1445–1447, 1996. View at Google Scholar - J. A. Armstrong, N. Bloembergen, J. Ducuing, and P. S. Pershan, “Interactions between light waves in a nonlinear dielectric,”
*Physical Review*, vol. 127, no. 6, pp. 1918–1939, 1962. View at Publisher · View at Google Scholar - F. M. Pigozzo, E. Autizi, A. D. Capobianco, N. Argiolas, M. Bazzan, and C. Sada, “A novel configuration for phase-matched second-harmonic generation in LiNbO3 waveguides,”
*IEEE Photonics Technology Letters*, vol. 19, no. 8, pp. 553–555, 2007. View at Publisher · View at Google Scholar - M. M. Fejer, G. A. Magel, D. H. Jundt, and R. L. Byer, “Quasi-phase-matched second harmonic generation: tuning and tolerances,”
*IEEE Journal of Quantum Electronics*, vol. 28, no. 11, pp. 3631–2654, 1992. View at Google Scholar · View at Scopus - D. Feng, N. B. Ming, J. F. Hong et al., “Enhancement of second-harmonic generation in LiNbO
_{3}crystals with periodic laminar ferroelectric domains,”*Applied Physics Letters*, vol. 37, no. 7, pp. 607–609, 1980. View at Publisher · View at Google Scholar · View at Scopus - M. Houé and P. D. Townsend, “Thermal polarization reversal of lithium niobate,”
*Applied Physics Letters*, pp. 2667–2669, 1995. View at Google Scholar · View at Scopus - Yamamoto and Mizuuchi, “Blue-light generation by frequency doubling of a laser diode in a periodically domain-inverted LiTaO
_{3}waveguide,”*IEEE Photonics Technology Letters*, vol. 4, no. 5, pp. 435–437, 1992. View at Publisher · View at Google Scholar - S. Miyazawa, “Ferroelectric domain inversion in Ti-diffused LiNbO
_{3}optical waveguide,”*Journal of Applied Physics*, vol. 50, no. 7, pp. 4599–4603, 1979. View at Publisher · View at Google Scholar - C. Restoin, C. Darraud-Taupiac, J. L. Decossas, J. C. Vareille, and J. Hauden, “Ferroelectric-domain-inverted gratings by electron beam on LiNbO
_{3},”*Materials Science in Semiconductor Processing*, vol. 3, no. 5-6, pp. 405–407, 2000. View at Publisher · View at Google Scholar · View at Scopus - H. Ito, C. Takyu, and H. Inaba, “Fabrication of periodic domain grating in LiNbO
_{3}by electron beam writing for application of nonlinear optical processes,”*Electronics Letters*, vol. 27, no. 14, pp. 1221–1222, 1991. View at Google Scholar - M. Fujimura, K. Kintaka, T. Suhara, and H. Nishihara, “Blue light generation in LiNbO
_{3}waveguide SHG device with first order domain-inverted grating formed by EB scanning,”*Electronics Letters*, vol. 28, no. 20, pp. 1868–1869, 1992. View at Google Scholar - P. W. Haycock and P. D. Townsend, “A method of poling LiNbO
_{3}and LiTaO_{3}below T_{c},”*Applied Physics Letters*, vol. 48, no. 11, pp. 698–700, 1986. View at Publisher · View at Google Scholar · View at Scopus - M. Yamada, N. Nada, M. Saitoh, and K. Watanabe, “First-order quasi-phase matched LiNbO
_{3}waveguide periodically poled by applying an external field for efficient blue second-harmonic generation,”*Applied Physics Letters*, vol. 62, no. 5, pp. 435–436, 1993. View at Publisher · View at Google Scholar · View at Scopus - J. Webjorn, V. Pruneri, P. S. J. Russell, J. R. M. Barr, and D. C. Hanna, “Quasi-phase-matched blue light generation in bulk lithium niobate, electrically poled via periodic liquid electrodes,”
*Electronics Letters*, vol. 30, no. 11, pp. 894–895, 1994. View at Publisher · View at Google Scholar · View at Scopus - M. Sato, P. G. R. Smith, and D. C. Hanna, “Contact electrode method for fabricating bulk periodically poled LiNbO
_{3},”*Electronics Letters*, vol. 34, no. 7, pp. 660–661, 1998. View at Google Scholar · View at Scopus - Y. J. Ding, S. J. Lee, and J. B. Khurgin, “Transversely pumped counterpropagating optical parametric oscillation and amplification,”
*Physical Review Letters*, vol. 75, no. 3, pp. 429–432, 1995. View at Publisher · View at Google Scholar - C. Conti, G. Assanto, and S. Trillo, “Cavityless oscillation through backward quasi-phase-matched second-harmonic generation,”
*Optics Letters*, vol. 24, no. 16, pp. 1139–1141, 1999. View at Google Scholar - K. Gallo, P. Baldi, M. De Micheli, D. B. Ostrowsky, and G. Assanto, “Cascading phase shift and multivalued response in counterpropagating frequency-nondegenerate parametric amplifiers,”
*Optics Letters*, vol. 25, no. 13, pp. 966–968, 2000. View at Google Scholar - A. C. Busacca, C. L. Sones, R. W. Eason, and S. Mailis, “First-order quasi-phase-matched blue light generation in surface-poled Ti:indiffused lithium niobate waveguides,”
*Applied Physics Letters*, vol. 84, no. 22, pp. 4430–4432, 2004. View at Publisher · View at Google Scholar - A. C. Busacca, C. L. Sones, V. Apostolopoulos, R. W. Eason, and S. Mailis, “Surface domain engineering in congruent lithium niobate single crystals: a route to submicron periodic poling,”
*Applied Physics Letters*, vol. 81, no. 26, pp. 4946–4948, 2002. View at Publisher · View at Google Scholar - G. D. Landry and T. A. Maldonado, “Counterpropagating quasi-phase matching: a generalized analysis,”
*Journal of the Optical Society of America B*, vol. 21, no. 8, pp. 1509–1520, 2004. View at Publisher · View at Google Scholar - A. C. Busacca, A. C. Cino, S. Riva-Sanseverino, M. Ravaro, and G. Assanto, “Silica masks for improved surface poling of lithium niobate,”
*Electronics Letters*, vol. 41, no. 2, pp. 92–93, 2005. View at Publisher · View at Google Scholar · View at Scopus - U. K. Sapaev and G. Assanto, “Femtosecond pulse synthesis by efficient second-harmonic generation in engineered quasi phase matching gratings,”
*Optics Express*, vol. 15, no. 12, pp. 7448–7457, 2007. View at Publisher · View at Google Scholar - U. K. Sapaev and G. Assanto, “Efficient high-harmonic generation in engineered quasi-phase matching gratings,”
*Optics Express*, vol. 16, no. 1, pp. 18370–18375, 2008. View at Publisher · View at Google Scholar - M. Conforti, C. De Angelis, U. K. Sapaev, and G. Assanto, “Pulse shaping via backward second harmonic generation,”
*Optics Express*, vol. 16, no. 3, pp. 2115–2121, 2008. View at Publisher · View at Google Scholar - U. K. Sapaev and G. Assanto, “Engineered quasi-phase matching for multiple parametric generation,”
*Optics Express*, vol. 17, no. 5, pp. 6765–6770, 2009. View at Publisher · View at Google Scholar - G. Assanto, “Quadratic cascading: effects and applications,” in
*Beam Shaping and Control with Nonlinear Optics*, F. Kajzar and R. Reinisch, Eds., B369, pp. 341–374, Plenum Press, New York, NY, USA, 1997. View at Google Scholar - G. Assanto and G. I. Stegeman, “Simple physics of quadratic spatial solitons,”
*Optics Express*, vol. 10, no. 9, pp. 388–396, 2002. View at Google Scholar - G. Leo, A. Amoroso, L. Colace, G. Assanto, R. V. Roussev, and M. M. Fejer, “Low-threshold spatial solitons in reverse-proton-exchanged periodically poled lithium niobate waveguides,”
*Optics Letters*, vol. 29, no. 15, pp. 1778–1780, 2004. View at Publisher · View at Google Scholar - C. Conti, E. D'Asaro, S. Stivala, A. Busacca, and G. Assanto, “Parametric self-trapping in the presence of randomized quasi phase matching,”
*Optics Letters*, vol. 35, no. 22, pp. 3760–3762, 2010. View at Publisher · View at Google Scholar - S. Stivala, A. C. Busacca, A. Pasquazi, R. L. Oliveri, R. Morandotti, and G. Assanto, “Random quasi-phase-matched second-harmonic generation in periodically poled lithium tantalate,”
*Optics Letters*, vol. 35, no. 3, pp. 363–365, 2010. View at Publisher · View at Google Scholar - A. Pasquazi, A. Busacca, S. Stivala, R. Morandotti, and G. Assanto, “Nonlinear disorder mapping through three-wave mixing,”
*IEEE Photonics Journal*, vol. 2, no. 1, pp. 18–28, 2010. View at Publisher · View at Google Scholar - J. S. Pelc, C. R. Phillips, D. Chang, C. Langrock, and M. M. Fejer, “Efficiency pedestal in quasi-phase-matching devices with random duty-cycle errors,”
*Optics Letters*, vol. 36, no. 6, pp. 864–866, 2011. View at Publisher · View at Google Scholar - S. Stivala, F. Buccheri, L. Curcio, R. L. Oliveri, A. C. Busacca, and G. Assanto, “Features of randomized electric-field assisted domain inversion in lithium tantalate,”
*Optics Express*, vol. 19, no. 25, pp. 25780–25785, 2011. View at Google Scholar - G. Nava, P. Minzioni, I. Cristiani, et al., “Integrated frequency shifter in a periodically poled lithium tantalate waveguide,”
*Electronics Letters*, vol. 46, no. 25, pp. 1686–1688, 2010. View at Google Scholar - S. Stivala, A. Pasquazi, L. Colace et al., “Guided-wave frequency doubling in surface periodically poled lithium niobate: competing effects,”
*Journal of the Optical Society of America B*, vol. 24, no. 7, pp. 1564–1570, 2007. View at Google Scholar - M. Cherchi, S. Stivala, A. Pasquazi et al., “Second-harmonic generation in surface periodically poled lithium niobate waveguides: on the role of multiphoton absorption,”
*Applied Physics B*, vol. 93, no. 2-3, pp. 559–565, 2008. View at Publisher · View at Google Scholar - A. C. Busacca, E. D'Asaro, A. Pasquazi, S. Stivala, and G. Assanto, “Ultraviolet generation in periodically poled lithium tantalate waveguides,”
*Applied Physics Letters*, vol. 93, no. 12, Article ID 121117, 2008. View at Publisher · View at Google Scholar - J. U. Kang, Y. J. Ding, W. K. Burns, and J. S. Melinger, “Backward second-harmonic generation in periodically poled bulk LiNbO
_{3},”*Optics Letters*, vol. 22, no. 12, pp. 862–864, 1997. View at Google Scholar - X. Gu, R. Y. Korotkov, Y. J. Ding, J. U. Kang, and J. B. Khurgin, “Backward second-harmonic generation in periodically poled lithium niobate,”
*Journal of the Optical Society of America B*, vol. 15, no. 5, pp. 1561–1566, 1998. View at Google Scholar - X. Gu, M. Makarov, Y. J. Ding, J. B. Khurgin, and W. P. Risk, “Backward second-harmonic and third-harmonic generation in a periodically poled potassium titanyl phosphate waveguide,”
*Optics Letters*, vol. 24, no. 3, pp. 127–129, 1999. View at Google Scholar - X. Mu, I. B. Zotova, Y. J. Ding, and W. P. Risk, “Backward second-harmonic generation in submicron-period ion-exchanged KTiOPO
_{4}waveguide,”*Optics Communications*, vol. 181, no. 1, pp. 153–159, 2000. View at Publisher · View at Google Scholar - S. Stivala, A. C. Busacca, L. Curcio, R. L. Oliveri, S. Riva-Sanseverino, and G. Assanto, “Continuous-wave backward frequency doubling in periodically poled lithium niobate,”
*Applied Physics Letters*, vol. 96, no. 11, Article ID 111110, 2010. View at Publisher · View at Google Scholar - A. C. Busacca, C. A. Santini, S. Riva-Sanseverino et al., “Surface periodic poling in congruent lithium tantalate,”
*Electronics Letters*, vol. 42, no. 9, pp. 546–547, 2006. View at Publisher · View at Google Scholar - M. Bazzan, C. Sada, N. Argiolas et al., “High resolution x-ray investigation of periodically poled lithium tantalate crystals with short periodicity,”
*Journal of Applied Physics*, vol. 106, no. 10, Article ID 104121, 2009. View at Publisher · View at Google Scholar - A. Busacca, M. Cherchi, S. Riva Sanseverino et al., “Surface periodic poling in lithium niobate and lithium tantalate,” in
*Proceedings of the 4th IEEE/LEOS Workshop on Fibres and Optical Passive Components (WFOPC '05)*, pp. 126–130, June 2005. View at Publisher · View at Google Scholar - L. Chanvillard, P. Aschiéri, P. Baldi et al., “Soft proton exchange on periodically poled LiNbO
_{3}: a simple waveguide fabrication process for highly efficient nonlinear interactions,”*Applied Physics Letters*, vol. 76, no. 9, pp. 1089–1091, 2000. View at Google Scholar - K. El Hadi, M. Sundheimer, P. Aschieri et al., “Quasi-phase-matched parametric interactions in proton-exchanged lithium niobate waveguides,”
*Journal of the Optical Society of America B*, vol. 14, no. 11, pp. 3197–3203, 1997. View at Google Scholar - A. C. Busacca, E. D'Asaro, S. Riva-Sanseverino, and G. Assanto, “Stable proton exchanged waveguides in lithium tantalate,”
*IEEE Photonics Technology Letters*, vol. 20, no. 24, pp. 2126–2128, 2008. View at Publisher · View at Google Scholar - M. De Micheli, D. B. Ostrowsky, J. P. Barety et al., “Crystalline and optical quality of proton exchanged waveguides,”
*Journal of Lightwave Technology*, vol. 4, no. 7, pp. 743–745, 1985. View at Google Scholar - A. C. Busacca, S. Stivala, L. Curcio et al., “Soft proton exchanged channel waveguides in congruent lithium tantalate for frequency doubling,”
*Optics Express*, vol. 18, no. 25, pp. 25967–25972, 1986. View at Publisher · View at Google Scholar - J. M. White and P. F. Heidrich, “Optical waveguide refractive index profiles determined from measurement of mode indices: a simple analysis,”
*Applied Optics*, vol. 15, no. 1, pp. 151–155, 1976. View at Google Scholar - M. Marangoni, M. Lobino, R. Ramponi, E. Cianci, and V. Foglietti, “High quality buried waveguides in stoichiometric LiTaO
_{3}for nonlinear frequency conversion,”*Optics Express*, vol. 14, no. 1, pp. 248–253, 2006. View at Publisher · View at Google Scholar - A. C. Busacca, R. L. Oliveri, A. C. Cino, S. Riva-Sanseverino, A. Parisi, and G. Assanto, “Ultraviolet quasi-phase-matched second harmonic generation in surface periodically poled lithium niobate optical waveguides,”
*Laser Physics*, vol. 17, no. 6, pp. 884–888, 2007. View at Publisher · View at Google Scholar - M. Horowitz, A. Bekker, and B. Fischer, “Broadband second-harmonic generation in ${\text{Sr}}_{\text{x}}{\text{Ba}}_{\text{1-x}}{\text{Nb}}_{\text{2}}{\text{O}}_{\text{6}}$ by spread spectrum phase matching with controllable domain gratings,”
*Applied Physics Letters*, vol. 62, no. 21, 1993. View at Google Scholar - K. Gallo, G. Assanto, and G. I. Stegeman, “Efficient wavelength shifting over the erbium amplifier bandwidth via cascaded second order processes in lithium niobate waveguides,”
*Applied Physics Letters*, vol. 71, no. 8, pp. 1020–1022, 1997. View at Google Scholar